Oxidation of cyclohexene with H2O2 over imogolite in acetic acid as a solvent. Reaction condition: temperature 50 °C, time 6h, imogolite 100 mg 1-ol : 2-cyclohexene-1-ol, trans-diol : trans-1,2-cyclohexanediol, cis-diol: 1,2-cyclohexanediol
Imogolite is a hydrated aluminosilicate with a unique tubular structure, which is found in volcanic ash soil and is shown in Figure 1. It was first discovered in glassy volcanic ash soil in Japan and was named after the soil in Hitoyoshi, Kumamoto Prefecture . Its chemical composition is (OH)3Al2O3Si(OH).
The tubular structure of imogolite was proposed by Cradwick et al.  based on results from electron diffraction observation and is shown in figure 2. The tube wall consists of a single continuous Al(OH)3 (gibbsite) sheet and orthosilicate anions (O3SiOH groups) associated with each vacant octahedral site of the gibbsite sheet. The imogolite has an outer diameter of ca. 2 nm and an inner diameter of ca. 1 nm.
Recently, imogolite has drawn a new attention as a new nano-material because of its unique nano-scale tubular structure similar to that of a single-walled carbon nanotube . Studies on synthesis [4-9], mechanisms of formation , structural evolution [11, 12], stability [13, 14], electronic states [14, 15] and application have been carried out. Proposed applications, such as a polymer composite [16,17], a fuel gas storage , an absorbent , an exchange material for heat pump system , a humidity-controlling material  and an anti-deweling material  have been discussed.
Application as a catalyst or a catalyst support also attracts attention because it is expected to have a shape-selective characteristic property as molecular sieving zeolites due to its unique tubular structure. However, few investigations [21, 22] have been reported using natural imogolite as a catalyst because the extraction of pure imogolite from the soil is difficult and time consuming . Therefore, synthesis of imogolite has become necessary in order to utilize it as a functional material.
We synthesized imogolite containing Fe3+ ions (Fe-imogolite) using NaSiO4, FeCl3 and AlCl3 to investigate its catalytic properties . Because of its chemical stability, an incorporation of another element is necessary to generate a chemical function. We found that it served as a catalyst of liquid-phase oxidation reactions of some hydrocarbons.
In this chapter, the synthetic methods, characterization and the general properties of imogolite is described at first. And then the characterization and catalytic properties of Fe-imogolite obtained from our researches is described.
2. Synthetic imogolite
In the latter half of the 1970's, synthesis of imogolite was succeeded from a dilute solution. Recently, various synthesis methods have been investigated and many characterizations have been carried out. In this section, synthesis methods, structural characterization and catalytic properties of synthetic imogolite are described.
2.1. Synthesis method of imogolite
Farmer et al. reported  the synthesis method of imogolite in 1977. Imogolite was synthesized from a dilute solution containing of hydroxyaluminum cations (2.4 mmol L-1) and orthosilicic acid (1.4 mmol L-1). Afterward, the solution was adjusted to pH 5 with sodium hydroxide, 1 mmol L-1 of hydrochloric acid solution and 2 mmol L-1 of acetic acid. Imogolite was obtained in this solution by heating it near the boiling point. Wada et al.  later also investigated the effects of Al-to-OH- (as sodium hydroxide) ratio to synthesizing imogolite and allophane using a dilute inorganic solution.
A diluted inorganic solution is necessary to form imogolite in these methods, because preventing the condensation of orthosilicic acid and the formation inhibition of it by anions is important to form the nanotube structure. However, it is difficult to obtain a large sample. Suzuki et al.  developed a synthetic method of producing imogolite using a concentrated inorganic solution. Sodium orthosilicate was used as a starting material to prevent the condensation of orthosilicic acid. Furthermore, a desalination process is carried out by centrifugation. We have synthesized Fe containing imogolite based on improving Suzuki’s method which will be described below in detail.
More recently, new synthesis methods of imogolite have been reported. Levard et al.  synthesized it from a decimolar concentration solution at 95 °C for 60 days. Abidin et al.  proposed a new supplying method of a silicon source using colloidal silica for the synthesis of imogolite.
2.2. Characterization of imogolite
Transmission electron microscopy (TEM) or scanning electron microscopy (SEM) is used mostly in order to observe the morphology and structure of imogolite nanotubes. Figure 3 shows an SEM image of synthetic imogolite.
Bursill et al.  have observed the various aggregations of them such as randomly oriented single tube, close-packed arrays or fiber bundles by high resolution TEM.
On the other hand, atomic force microscopy (AFM) is a powerful tool to investigate them under ambient conditions. The tapping-mode AFM especially shows the morphological features of the synthetic imogolite clearly [26, 27]. Figure 4 shows the tapping mode AFM image of synthetic imogolite. Fibrous materials with a length of 100 - 1000 nm can be observed in this image.
2.2.2. Structural characterization
The analytical methods, such as X-ray diffraction (XRD), infrared (IR) spectroscopy and solid state nuclear magnetic resonance (NMR) are used in order to identify or characterize imogolite. In this section, the features of imogolite obtained using these analytical methods are mentioned.
The XRD profiles which were obtained by Cu Kα irradiation are given in Figure 5. Imogolite is characterized by three broad peaks in the low angle region. There are three peaks at 2θ = 5.1°, 11° and 15.6° in the XRD profile of natural imogolite and at 2θ = 4.6°, 9.6° and 14.3° in that of synthetic imogolite. The difference in peak position is due to the difference in the diameter of a tube of a natural and synthetic imogolite [7, 24]. The diameter of 1.8 - 2.2 nm in natural imogolite  and 2.7 - 3.2 nm in synthetic imogolite  were reported.
FT-IR spectra of Natural and synthetic imogolite, which are shown in figure 6, have a characteristic absorption that appears as a doublet at around 1000 cm-1. These absorptions are attributed to Si-O (higher frequency) and Si-O-Al (lower frequency) stretching . These samples also have some absorption bands in the region from 400 cm-1 to 750 cm-1. The absorption bands at 685 cm-1, 563 cm-1 and 427 cm-1 in natural imogolite arise from various Al-O vibrations .
Imogolite is also characterized by 29Si and 27Al solid state NMR [30-34]. Magic angle spinning (MAS) techniques are used in general in order to obtain a high resolution NMR spectrum of sold state. Goodman et al.  have carried out 29Si and 27Al MAS NMR measurements of synthetic imogolite. The peak is observed at -78.8 ppm in 29Si MAS NMR spectrum of it as well as natural imogolite. Barron et al.  have shown that the observed chemical shift of natural imogolite is consistent with silicon tetrahedra which are isolated by coordination through oxygen with three aluminum atoms and one proton. On the other hand, 27Al MAS NMR spectrum of imogolite has one peak at 0 ppm and it is attributed to the six coordinated octahedral Al3+ species [31-34].
2.1.3. Thermal transformation of synthetic imogolite
The differential thermal analysis (DTA) and thermo gravimetric analysis (TGA) traces of synthetic imogolite are shown in Figure 7. Two broad endothermic peaks with a weight loss and an exothermic peak without a weight change were observed.
MacKenzie et al.  investigated thermal transformation of natural imogolite by using DTA-TGA, 29Si MAS NMR and 27Al MAS NMR and proposed the structural models which were changed by heating. The results of DTA-TGA showing thermal transformation of imogolite are explained based on their literature. The endothermic peaks at 110 °C and 400 °C were attributed to the loss of adsorbed water and dehydroxylation, respectively. Amorphism of imogolite occurred by these dehydroxylations. The exothermic peak at 950 °C was attributed to crystallization to mullite (Al6Si2O13). Donkai
2.1.4. Catalytic properties
It has been known that imogolite has surface acidity . The acid strength of it is increased by heat treatment. Natural imogolite calcined at various temperatures were used as catalysts for the isomerization of 1-butene . This reaction proceeded effectively over samples calcined at 400 °C. The decomposition reaction of organic peroxides also was investigated using Cu2+ loaded imogolite calcined at 500 °C. Furthermore, it was mentioned that imogolite calcined at temperature up to 750 °C exhibited the shape selective adsorption. Bonelli et al.  have studied
We have investigated the acidic property of imogolite without heat treatment . At first, we attempted an isomerization reaction of α-pinene on synthetic imogolite. It is known that the isomerization products of α-pinene depend on the acid or base property of the catalyst. In the case of acid catalysts, α-pinene isomerize to limonene, camphene and tricyclene . Prior to the reaction imogolite was dried at 120 °C for 12 hours. The isomerization reaction of α-pinene was carried out at 80 °C for 3 hours or 24 hours using an evacuated batch reactor. In a typical experiment, the reactor was loaded with 12.6 mmol of α-pinene and 50 mg of catalyst. The α-pinene did not react on it. It was reported that imogolite had a weak acid property, however it was not detected in this reaction.
Although isomerization of α-pinene did not occurre, some oxidation products of it were detected slightly. So the oxidation reaction of cyclohexene using hydrogen peroxide was carried out to test the possibility as an oxidation catalyst.
In a typical catalytic experiment for oxidation , the reaction was carried out by using 25 mmol of cyclohexene, 25 mmol of H2O2 (30 wt%) and 30 ml of acetic acid or acetonitrile as a solvent with 100 mg of catalyst under being stirred at 50 °C. The results of the oxidation reaction of cyclohexene with H2O2 are listed in Table 1. Without a catalyst the oxidation products such as trans-1,2-cyclohexanediol, cis-1,2-cyclohexanediol and 2-cyclohexene-1-ol were observed using acetic acid as solvent. With imogolite the yield of these oxidation products was increased, but the selectivity was almost the same as the control experiment. This result indicates that imogolite has the potential of concentration and acts as a field of reaction to increase collision frequency.
In the case of using acetonitrile as the solvent, the oxidation products were not detected for 27 hours of reaction time. In the case of imogolite, 2-cyclohexene-1-ol and 1,2-epoxycyclohexene were produced with 0.5 % and 0.8 % yields, respectively. This results shows that imogolite has the possibility as an oxidation catalyst.
Although we found the new possibility of synthetic imogolite as an oxidation catalyst, a chemical modification of imogolite like an introduction of Fe3+ ion was necessary to promote the reaction because imogolite is chemically stable. In this section, our results of the synthetic method, characterization and catalytic test of Fe-imogolite are described.
3.1. Synthesis of Fe-imogolite
We prepared 100 mL of 0.15 mol L-1 aqueous solutions consist of FeCl3 and AlCl3 with x = 0.05 (x = Fe/Al+Fe, atomic ratio). Another way of saying, 0.00075 mol FeCl3・6H2O and 0.01425 mol AlCl3・6H2O were dissolved in 100 mL of water.
100 mL of 0.1 mol L-1 Na4SiO4 aqueous solution was prepared.
Na4SiO4 aqueous solution was added to AlCl3 and FeCl3 mixture and the solution was stirred for 90 minutes.
0.1 mol L-1 NaOH aqueous solution was added to the solution consist of Na4SiO4, FeCl3 and AlCl3 at the rate of 1.0 mL min-1 under stirring until the pH of the mixture become 5.5.
The salt-free precursor was obtained from thick solution by centrifugal separation three times.
It was dispersed in 2 L of water and 40 mL of 0.1 mol L-1 HCl was added.
The solution was stirred for two hours at room temperature.
It was aged at 100 °C for 40 hours.
This aging solution was dialyzed and then dried at 100 °C for two days.
The film-like Fe-imogolite was obtained.
3.2. Characterization of Fe-imogolite
Fe containing samples with x = 0, 0.05, 0.1 were prepared in order to survey the effect of Fe3+ contents in starting solutions to formation of imogolite nanotubes,. The XRD profiles and IR spectra of these samples are shown in Figure 8.
As mentioned above, imogolite (x = 0) was characterized by three broad peaks in the low angle region of the XRD profile and a doublet at around 1000 cm-1 in the FT-IR spectrum. In the case of x = 0.1, it lacks the three broad peaks in XRD and a doublet in FT-IR, meaning the sample does not have the imogolite structure. In the case of x=0.05, the XRD profile and FT-IR spectrum were similar to the imogolite. The intensity of the three broad peaks is weaker than that of imogolite because XRD measurements were carried out using Cu Kα irradiation. The color and the profiles of XRD and FT-IR indicate the sample with x=0.05 is considered Fe containing imogolite and is thus called Fe-imogolite.
In order to investigate the state of iron ions in Fe-imogolite, it was compared with the Fe3+ ion adsorbed on imogolite The adsorbed Fe3+ ions sample was prepared by adsorbing FeCl3 onto imogolite from aqueous solution of FeCl3 and is called FeCl3/imogolite. These samples are both reddish brown and the absorption bands of them were observed at the region above 15,000 cm-1 in diffuse reflectance ultraviolet visible (UV-VIS) spectra (Figure 9). The absorption bands of Fe3+ in many minerals are observed in this region.
It has been known that when the tetrahedral species of Fe3+ exist, the pre-edge peak appears strongly in X-ray absorption near edge structure (XANES) spectra. XANES spectra of Fe K-edge (7.111 keV) are shown in Figure 10. The pre-edge peak was not observed in the spectrum of Fe-imogolite nor FeCl3/imogolite or Fe2O3. Thus it is clear that the state of iron in Fe-imogolite is octahedral Fe3+ ion from the results of UV-VIS and XANES spectra.
Figure 11 shows their Fourier transforms (FT) spectra of Fe-imogolite, FeCl3/imogolite and Fe2O3. FT spectrum as radial structure function was obtained by Fourier transformation of
The tapping mode AFM image of Fe-imogolite is shown in figure 12 . The fibrous morphology was observed similar to the synthetic imogolite. It was found that the tube diameter was almost uniform and estimated to be 2.2-2.4 nm from section analysis.
3.3. Oxidation of hydrocarbons using Fe-imogolite catalyst
3.3.1. Oxidation of cyclohexene [ 23]
The oxidation of cyclohexene was carried out using cyclohexene, H2O2 and acetonitrile as a solvent with catalysts under being stirred at 50 °C for 24 hours. No product was detected without a catalyst. In the case of imogolite, 2-cyclohexene-1-ol and 1,2-epoxycyclohexane (EP) were produced slightly as stated above. EP was also detected in separate experiments using gibbsite, boehmite and Al2O3 as catalysts. Mandelli et al.  have reported the epoxidation of cyclohexene using H2O2 over Al2O3. It was attributed that these oxidation compounds may be produced on the outer surface of the imogolite. The oxidation reaction was promoted by Fe-imogolite and not only alcohol and epoxy compounds but trans-1,2-cyclohexanediol, cis-1,2-cyclohexanediol and 2-cyclohexene-1-one were also obtained as products.
Phenol is one of the most important chemicals in the fields of fiber and medicine manufacturing. More than 90% of phenol is produced by the cumen process, which is a three-step process and produces acetone as a by-product. The development of a one-step process for phenol synthesis by the direct oxidation of benzene is important when concerned with green chemistry as an environment-friendly technique. It was found that benzene or other aromatic hydrocarbons were oxidized by H2O2 over Fe-imogolite. These results are described.
The reaction of benzene was carried out using 2 mmol of benzene, 11 mmol of H2O2 and 10 mL of acetonitrile as a solvent with 100 mg of catalyst under being stirred at 60 °C. The products were analyzed by GC-MASS. The conversion of H2O2 was determined by a volumetric analysis with KMnO4.
Figure 13 shows the results of oxidation reactions of benzene using H2O2 and compounds containing Fe. None of the oxidation products were detected without catalysts and with FeCl3/imogolite, Fe2O3 (hematite) and α-FeOOH (goethite) as a catalyst. It is an interesting finding that only phenol was obtained as an oxidation product by GC-Mass using Fe-imogolite .
The oxidation reactions of benzene using four solvents were examined. The results are summarized in Table 2. None of oxidation products were detected in the case of acetic acid and propionic acid as a solvent. It was found that acetonitrile was the most effective for this reaction among the examined solvents. Although the solution turned palish yellow using acetonitrile as a solvent, after the reaction the absorption due to the Fe3+ ion was not detected in UV-VIS absorption spectrum. It was suggested that the origin of the coloring could be phenolic tars that could not detected by GC-Mass. A conversion of H2O2 was high with all solvent and H2O2 efficiency was 2 % using acetonitrile as a solvent. Thus, the decomposition of H2O2 was only caused by using other solvents except for acetonitrile.
The results of the oxidation reaction of aromatic hydrocarbons using Fe-imogolite as a catalyst are summarized in Table 3 . Hydroquinone and catechol were produced as products from phenol by the oxidation with H2O2.
|Solvent||Conversion / %||Yield of|
Phenol / %
When the side chain is a hydrocarbon group such as methyl, both the benzene ring and the side chain group were oxidized. It was found that the side chain group was more easily oxidized.
Monfared and Amouei  have reported direct oxidation reactions of benzene or some aromatic hydrocarbon compounds over Fe3+ loaded Al2O3 (Fe3+-Al2O3) with H2O2 in acetonitrile. In their system, however,
3.3.3. Oxidation of cyclohexane [42, 43]
Oxidation of cycloxane under mild conditions have been very interesting and have attempted widely . Since the oxidation takes place not only on aromatic rings but on methyl groups by H2O2 in acetonitrile over Fe-imogolite catalysts, other organic compounds such as saturated hydrocarbons could be oxidized under this reaction condition. We examined the oxidation of cyclohexane using this catalyst.
|Reactant||Products (Yield* / %)|
benzoic acid (71.7)
The reaction of cyclohexane was carried out using 2 mmol of cyclohexane, 10 mmol of H2O2 and 10 ml of acetonitrile as a solvent with 50 mg of catalyst under being stirred at 60 °C for 3 hours. The products were analyzed by GC-Mass and GC with FID detector. The oxidation products were hardly detected without catalysts. With Fe-containing imogolite as a catalyst, this reaction was promoted and three oxidation products were created. Two compounds were easily identified by retention time of standard reagents such as cyclohexanone and cyclohexanol among these products. Another is speculated as cyclohexyl hydroperoxide from fragmentation patterns in the mass spectrum. It was reported  that cyclohexyl hydroperoxide was prepared efficiently and selectively using cyclohexane and H2O2 over Fe3+ ion-changed montmorillonite. We identified one of the oxidation products as cyclohexyl hydroperoxide by the compound obtained following this examination. The conversion of cyclohexane was ca. 25%.
The cyclohexyl hydroperoxide was produced immediately as soon as the reaction started. Additionally, it was detected only in oxidation reactions with Fe2O3 or α-FeOOH as a catalyst. It was found that cyclohexanone and cyclohexanol were produced via cyclohexyl hydroperoxide as an intermediate which was obtained by reacting cyclohexane and H2O2 (Figure 14).
Fe-imogolite was synthesized using Na4SiO4, AlCl3 and FeCl3 with the atomic ratio Fe / (Al+Fe) = 0.05 and applied as a liquid-phase oxidation catalyst with hydrogen peroxide.
The XRD profile and FT-IR spectrum of this material were similar to the synthetic imogolite. AFM images showed fibrous morphology with ca. 2 nm of diameter. UV-VIS and X-ray absorption spectra revealed the state of Fe3+ to be in the octahedral coordination. It was found that Fe-imogolite played as an oxidation catalyst of some hydrocarbons such as cyclohexane, benzene, phenol, toluene and cyclohexane with hydrogen peroxide. The oxidation reaction of cyclohexene was promoted by using Fe-imogolite instead of imogolite as a catalyst. It gave 2-cyclohexene-1-ol, 1,2-epoxycyclohexane, 1,2-cyclohexanediol and 2-cyclohexene-1-one as products. Phenol was produced by the oxidation reaction of benzene. The benzene ring in the aromatic hydrocarbons such as phenol, chlorobenzene, toluene and benzaldehyde was oxidized. Moreover, when the side-chain is a hydrocarbon group, side-chain group was also oxidized. It could be more easily oxidized than the benzene ring. Cyclohexyl hydroperoxide, Cyclohexanone and cyclohexanol were obtained as oxidation products of cyclohexane. It was clarified found that cyclohexanone and cyclohexanol were produced via cyclohexyl hydroperoxide. The possibility of Fe-imogolite as an oxidation catalyst is shown. However, its reaction mechanism has not been clarified yet. It is necessary to investigation the catalytic properties and the structure of Fe-imogolite further.
Yoshinaga N. Aomine S. 1962Imogolite in some Ando soils, Soil Sci. Plant Nutr. 8: 114−121.
Cradwick P. D. G. Farmer V. C. Rucell J. D. Masson C. R. Wada K. Yoshinaga N. 1972Imogolite, a Hydrated Aluminum Silicate of Tubular Structure Nature Phys. Sci. 240 187 189
Bursill L. A. Peng J. L. Burgeois L. N. 2000Imogolite: an aluminosilicate nanotube materials, Philos. Mag., 80 105 117
Koenderink G. H. Kluijtmans S. G. J. M. Philipse A. P. 1999On the Synthesis of Colloidal Imogolite Fibers, J. Colloid. Interface Sci. 216 429 431
Hu J. Kannangara G. S. K. Wilson M. A. Reddy N. 2004The fused silicate rote to protoimogolite and imogolite, J. Non-cryst. Solids, 347 224 230
Suzuki M. Ohashi F. Inukai K. Maeda M. Tomura S. 2000Synthesis of Allophane and Imogolite from Inorganic Solution- Influence of Co-Existing lon Concentration and Titration Rate on Forming Precursor-, Nendo Kagaku (J. Clay Sci. Soc. Japan), 40 1 14
Suzuki M. Inukai K. 2010Synthesis and Applications of Imogolite Nanotubes, in: Kijima T. editors, Inorganic and Metallic Nanotubular Materials, Topics in Applied Physics, 117: Springer 159 167 DOI:
Levard C. Masion A. Rose J. Doelsch E. Borschneck D. Dominici C. Ziarelli F. Bottero J. Y. 2009Synthesis of Imogolite Fibers from Decimolar Concentration at Low Temperature and Ambient Pressure: A Promising Route for Inexpensive Nanotubes, J. Am. Chem. Soc. 131 17080 17081
Abidin Z. Matsue N. Henmi T. 2008A New Method for Nano Tube Imogolite Synthesis, Jpn. J. Appl. Phys. 47 5079 5082
Mukherjee S. Bartlow V. M. Nair S. 2005Phenomenology of the Growth of Single-Walled Aluminosilicate and Aluminogermanate Nanotubes of Precise Dimensions, Chem. Mater., 17 4900 4909
Donkai N. Miyamoto T. Kokubo T. Tanei H. 1992Preparation of transparent mullite-silica film by heat-treatment of imogolite, J. Mater. Sci., 27 6193 6196
Mac Kenzie. K. J. D. Bowden M. E. Brown I. W. M. Meinhold R. H. 1989Structure and thermal transformations of imogolite studied by 29Si and 27Al high-resolution solid-state nuclear magnetic resonance, Clays Clay Miner. 37 317 324
Tamura K. And Kawamura. K. 2002Molecular Dynamics Modeling of Tubular Aluminum Silicate: Imogolite, J. Phys. Chem. B, 106 271 278
Luciana Guimarães. L. Andrey N. Enyashin A. N. Frenzel J. Heine T. Duarte H. A. Seifert G. 2007Imogolite Nanotubes: Stability, Electronic, and Mechanical Properties, ACS Nano, 1 362 368
Fernando Alvarez-Ramírez, 2007Ab initio simulation of the structural and electronic properties of aluminosilicate and aluminogermanate natotubes with imogolite-like structure, Phys. Rev. B 76 125421 125434
Yamamoto K. Otsuka H. Wada S. I. Sohn D. Takahara A. 2005Preparation and properties of [poly(methyl methacrylate)/imogolite] hybrid via surface modification using phosphoric acid ester, Polymer, 46 12386 12392
Yah W. O. Yamamoto K. Jiravanichanun N. Otsuka H. Takahara A. 2010Imogolite Reinforced Nanocomposites: Multifaceted Green Materials, Materials, 3 1709 1745 doi:10.3390/ma3031709.
Ohashi F. Tomura S. Akaku A. Hayashi S. Wada S. I. (200 2004Characterization of synthetic imogolite nanotubes as gas strage, J. Mater. Sci., 39 1799 1801
Ackerman W. C. Smith D. M. Huling J. C. Kim Y. H. Bailey J. K. Brinker C. J. 1993Gas/Vapor Adsorption in Imogolite: A Microporous Tubular Aluminosilicate, Langmuir, 9 1051 1057
Suzuki M. Ohashi F. Inukai K. Maeda M. Tomura S. Mizota T. 2001Hydration Enthalpy Measurement and Evaluation as Heat Exchangers of Allophane and Imogolite, J. Ceram. Soc. Japan, 109 681 685
Imamura S. Hayashi Y. Kajiwara K. Hoshino H. Kaito C. 1993Imogolite: A Possible New Type of Shape-Selective Catalyst, Ind. Eng. Chem. Res., 32 600 603
Imamura S. Kokubu K. Yamashita T. Okamoto Y. Kajiwara K. Kanai H. 1996Shape-Selective Copper Loaded Imogolite Catalyst, J. Catal., 160 137 139
Ookawa M. Inoue Y. Watanabe M. Suzuki M. Yamaguchi T. 2006Synthesis and Characterization of Fe containing Imogolite, Clay Sci., 12, Supplement 2 280 284
Farmer V. C. Fraser A. R. Tait J. M. 1977Synthesis of imogolite: A tubular aluminum silicate polymer, J. Chem. Soc. Chem. Comm., 13 462 463
Wada S. I. Eto A. Wada K. 1979Synthetic allophane and imogolite, J. Soil Sci., 30 347 355
Tani M. Liu C. Huang P. M. 2004Atomic force microscopy of synthetic imogolite, Geoderma, 118 209 220
Ohrai Y. Gozu T. Yoshida S. Takeuchi O. Iijima S. Shigekawa H. 2005Atomic force microscopy on imogolite, aluminosilicate nanotube, adsorbed on Au(111) surface, Jpn. J. Appl. Phys., 44 5397 5399
Mccutcheon A. Hu J. Kannangara G. S. K. Wilson M. A. Reddy N. 2005Si labelled nanoaluminosilicate imogolite, J. Non-Cryst. Solids, 351 1967 1972
Wada S. I. Wada K. 1982Effects of the substitution of germanium for silicon in imogolite, Clays Clay Miner., 30 123 128
Barron P. F. Wilson M. A. Campbell A. S. Frost R. L. 1982Detection of imogolite in soils using solid state 29Si NMR, Nature 299 616 618
Ildefonse P. Kirkpatrick R. J. Montez B. Calas G. Flank A. M. Lagarde P. 1994Investigated structure of imogolite using 27Al magic-angle-spinning (MAS) NMR and aluminum X-ray absorption near edge structure, Clay. Clay Min., 42 276 287
Chem. Minerals, Goodman B. A. Russell J. D. Montez B. Oldfield E. Kirkpatrick R. J. Structural studies. of imogolite. allophanes by. aluminum- silicon- nuclear magnetic. resonance spectroscopy. Phys 12 342 346
Hiradate S. Wada S. I. 2005Weathering process of volcanic glass to allophane determined by 27Al and 29Si solid-state NMR, Clay. Clay Min., 53 401 408
Hatakeyama M. Hara T. Ichikuni N. Shimazu S. 2011Characterization of Heat-Treated Synthetic Imogolite by 27Al MAS and 27Al MQMAS Solid-State NMR Bull. Chem. Soc. Jpn., 84 656 659
Henmi T. Wada K. 1974Surface acidity of imogolite and allopahne, Clay Minerals, 10 231 245
Bonelli B. Ilaria Bottero. I. Ballarini N. Passeri S. Cavani F. Garrone E. 2009IR spectroscopic and catalytic characterization of the acidity of imogolite-based systems, J. Catal., 264 15 30
Ookawa M. Onishi Y. Fukukawa S. Matsumoto K. Watanabe M. Yamaguchi T. Suzuki M. 2006Catalytic Property of Synthetic Imogolite, Nendo Kagaku (J. Clay Sci. Soc. Japan), 45 184 187
Ohnishi R. Tanabe K. Morikawa S. Nishizaki T. 1974Isomerization of 2-Pinene Catalyzed by Solid Acids, Bull. Chem. Soc. Jpn. 47 571 574
Ookawa M. Takata Y. Suzuki M. Inukai K. Maekawa T. Yamaguchi T. 2008Oxidation of aromatic hydrocarbons with H2O2 catalyzed by a nano-scale tubular aluminosilicate, Fe-containing imogolite, Res. Chem. Inter., 34 679 685
Mandelli D. van Vliet M. C. A. Sheldon R. A. Schuchardt U. 2001Alumina-catalyzed alkene epoxidation with hydrogen peroxide, Appl. Cat. A, 219 209 213
Monfared H. H. Amouei Z. 2004Hydrogen peroxide oxidation of aromatic hydrocarbons by immobilized iron(III), J. Mol. Cat. A, 217 161 164
Ookawa M. Nagamitsu Y. Oda M. Takata Y. Yamaguchi T. Maekawa T. 2008Catalytic properties of Fe-containing imogolite in cyclohexane oxidation, Interfaces Against Pollutions 2008 Programs & Abstracts: 24.
Ookawa M. Nagamitsu Yamaguchi. T. Maekawa T. 2007Oxidation of cyclohexane Catalyzed by Fe-containing imogolite, Abstracts ISSEM2007 International Symposium on Sustainable Energy & Materials: 47.
Schuchardt U. Cardoso D. Sercheli R. Pereira R. da Cruz. R. S. Guerreiro M. C. Mandelli D. Spinacé E. V. Pires E. L. 2000Cyclohexane oxidation continues to be a challenge, Appl. Cat. A 211 1 17
Ebitani K. Ide M. Mitsudome T. Mizugaki T. Kaneda K. 2002Creation of a chain-like cationic iron species in montmorillonite as a highly active heterogeneous catalyst for alkane oxygenations using hydrogen peroxide, Chem. Comm.: 690 691